Roller-Compacted Concrete Density:Principles and Practices
W A T E R R E S O U R C E S
One of the most common measurements used for quality control of earthfill placement is compacted density. The use ofdensity testing for the control of fill placement and as a keyindicator that material placed will meet specified parametershas broad application and a history of more than 50 years.
A key to design and construction using RCC is the applicationof testing procedures for both laboratory and field density thatis representative of in-place conditions. Several test methodsdeveloped over the last 20 years are described in this publica-tion. Also included is information on soil mechanics and concrete methodology aspects of RCC as well as a discussionon various standard compaction methods.
Basic Properties. In soil mechanics practice, the density of a soil is defined as the weight per unit volume. The typicalcomposition of a soil, subdivided into the three basic soilphasessolid, liquid (water), and gas (air)is shown inFigure 1. Various relationships and engineering properties arederived from these soil phases, for example, density, unitweight, porosity, degree of saturation, specific gravity, andwater content. Soil density is dependent on the relative volumeof solid particles and void spaces. The relative amount of void
volume in a soil mass can be expressed in terms of void ratio,or porosity: where the void ratio is defined as the ratio of thevolume of the voids (air and water) to the volume of the solidsin the soil mass, and porosity is defined as ratio of the volumeof voids to the total volume of the soil mass. Basic engineeringproperties in soil mechanics are commonly defined as follows:
V = total volume of soil massVs = volume of solid particlesVv = volume of void spaces (includes water and
air voids)Va = volume of air voidsVw = volume of water voidsW = total wet weight of soil massWs = dry weight of solidsWw = weight of water in soil masse = void ration = porosity, in percentA = percent air voids
= wet density (total unit weight of soil mass)= dry unit weight or density= unit weight of water
w = water or moisture content, in percentS = degree of saturationGa = apparent specific gravityGssd = saturated surface dry specific gravity
Figure 1. Relationship amongsoil phases:a) Visualization of a soil massb) Elements separated intophases of the soil mass.1
The definitions of the basic properties are expressed by the following formulas.
Total volume:V = Vs + Vv
Volume of voids:Vv = Va + Vw
Void ratio:e = Vv / Vs
Porosity:n = Vv / V x 100
Percent air voids:A = Va / V x 100
Degree of saturation:S = Vw / Vv
Total water content (oven dry):w = Ww / Ws
Density (total or wet):
Specific gravity (apparent):Ga = Wd / Ww
Figure 1 graphically shows the parameters that are used in the various equations.
Soil Compaction Tests for Determining Maximum Density/Optimum Water Content
There are two commonly used soil compaction tests for monitoringand controlling fill placement material. They are the standard Proctortest (ASTM D 698) and the modified Proctor test (ASTM D 1557).Both tests determine an optimum moisture content that results inthe maximum dry density unique to each material and the particularcompaction method. The two test methods differ in the amount ofenergy used in compacting the test specimens.
Experience has shown that the modified Proctor test is more suitable to roller-compacted concrete, due to the coarse nature ofRCC and the ability to achieve high compactive effort in the fieldthrough the use of large steel-drum vibratory compactors typicallyused on RCC projects. Both the standard and modified Proctor testswere developed for soils. The modified Proctor compaction test uses 56,000 ft-lbf/ft3 (2,700 kN-m/m3) versus 12,300 ft-lbf/ft3
(600 kN-m/m3) for the standard Proctor test. An important basis forthe Proctor compaction test, as stated in the test standards, is thatthe standards only apply to soil containing less than 30 % retainedon the 3/4 inch sieve. Because of the coarse nature of RCC mixtures,the Proctor compaction test procedures do not have direct applica-bility. Therefore, testing has been performed to explore the effectsthat the maximum size of aggregate, fines content, and cement andpozzolan contents could have on the compaction test. Tests byCasias et al.,3 Arnold et al.,4 Wong et al.,5 and Reeves and Yates,6have investigated various aspects of the compaction tests on RCC.
The modified Proctor test has several different performance methods.The current version (reapproved in 1998) includes Procedures A, B,and C (earlier versions included a Procedure D that has since been
discontinued, but is still referred to in some specifications). Themethod to be applied generally depends on the maximum particlesize of the soil sample and the quantity of fine gravel and materiallarger than 3/4 inch. In most cases Procedure C with a 6-inch diametermold, compared to 4-inch diameter molds for Procedures A and B,is used for RCC. The larger aggregates in RCC dictate the use of alarger mold to minimize the confining effect. The modified Proctortest consists of preparing a material at a moisture content and thencompacting a sample using a specified energy in a container ofknown volume. The compaction process expels air from the soil massby rearranging the particles to a denser configuration. The test continues with the compaction of the same material at differentmoisture contents and then plotting the results of dry density versusmoisture content. The result is a curve showing a distinct maximumdry density and optimum water content, as seen in Figure 2.
Experience with compaction control for earthfill placement hasshown that a material can be compacted to a high percentage (usually 95 %98 %) of the maximum dry density with commonlyavailable compaction equipment. Some variability inherently occursin the soil properties (e.g., changes in gradation or proportions ofsoil fractions, the specific gravity and/or absorption), and thechanges in soil properties may result in a different compaction curve.Consequently, a benefit of the modified Proctor compaction controlprocess is that the compaction curve automatically changes whensoil properties change naturally.
With compaction testing equipment, such as the nuclear densitygauge to measure in-place density, compaction in the field can becompared to the maximum density that can be achieved using themodified Proctor test. Comparing the in-place density in the fieldwith the maximum density achieved by the modified Proctor testprovides compaction control as a specified percent compaction andhas been used for field quality control for many RCC constructionprojects. However, as indicated in the following paragraph, place-ment of RCC at optimum moisture content (ASTM D1557) has resulted in a higher void content than is readily achieved for wellconsolidated RCC in the field. It should also be noted that fill controlusing the modified Proctor compaction test typically involves fillplacement and compaction on loose lift thickness of 8 inches to 10inches, in comparison with loose lift thickness up to 15 inches thatare common to RCC dam placements. As a result RCC is usuallyplaced at a water content above optimum moisture content (ASTMD1557), which provides more workability and transfer of energy forcompaction to the lower portion of the lift.
There are some other relevant aspects of the modified Proctor compaction test that are noteworthy; namely the concept of a zero-air-voids curve and the wet density of a material. Theoretically, thedry density of the material will parallel the zero-air-voids curve (asshown in Figure 2) that is unique for each material based on theapparent specific gravity of the material. As a porous material, soilhas an apparent specific gravity, which is defined as the ratio ofthe dry weight of a unit volume of soil (volume of solids plus volumeof voids) to the unit weight of water. The apparent specific gravity (Ga)is defined in ASTM C 127 as the ratio of the weight in air of a unitvolume of the impermeable portion of the aggregate to the weightin air of an equal volume of water. The zero-air-voids line is differentfrom the air content as determined in concrete practice. This difference isobvious when the wet density of the material from a modified
d = W V = / (1+ W)s /
= W / V
Proctor compaction test is plotted with the zero-air-voids line (seeFigure 2). In most material, the maximum wet density usually reachesa peak density at a higher water content than the maximum drydensity. This is due to the fact that with increasing water content, thevoids in the soil mass continue to be filled with water until the soilmass becomes too soft to sustain the compaction equipment. Athigher water contents, the soil mass contains more voids (air andwater), is less dense, and has increased plasticity (softness). Hencethe wet density curve begins to fall off. This can be complicated bythe absorption (both the percent of absorption and the absorptionrate) of the soil.
In order to demonstrate the properties described above, an exampleproblem will be used. With the definitions described above, the basicengineering properties of a soil (including an RCC mixture) can becalculated using soil mechanics. Example 1 below calculates variousengineering properties, given the apparent specific gravity of thematerial and the results from a modified Proctor test on an RCC mix-ture. General material properties of the soil aggregate used in thetest are summarized in Table 1.
Example 1: Assume one cubic foot (ft3) of RCC has a maximumwet density of 152.40 pounds per ft3 (pcf) and an apparent specific gravity (Ga) of 2.8. Using Figure 2, and an optimum moisture content of 7.0 %, a cement content of 412 pounds per cubic yard(pcy), and no pozzolan, the various engineering properties can becalculated as follows:
Ga = 2.80
Dry density curveMaximum dry density
Wet density curve
Ga = Apparent Specific Gravity160
1202 3 4 5 6 7
Moisture content, %
8 9 10 11 12
Zero Air Voids Curve
= 52.40 lb 42.43 lb= 9.97 lb
V =9.97 lb62.4 pcf
= 0.1598 ft
(cement) =12 lb
= 15.26 lb
V =15.26 lb
3.15 62.4 pcf= 0.0776 ft
V (soil) = Volume of the solids less
the volume of cement
W = 142.43 lb
V = 127.17 lb
2.8 62.4 pcf= 0.7279 ft
soil lb lb
15 26 127 17
( ) . .
Figure 2. Compaction curve of an RCC mixture (ASTM D 1557).
Roller-Compacted Concrete Density
Determine dry density:
= / (1+w)
= 142.43 pcf
Determine volume of constituents as shown in Figure 3:
Table 1 Material Properties for Example ProblemProperty Coarse Fine Weighted
Aggregate Aggregate Properties(> No. 4) (< No. 4)
Specific Gravity 2.69 2.95 2.80(Apparent)
Specific Gravity (Saturated Surface 2.63 2.85 2.72Dry)
Absorption 1.50 % 1.95 % 1.69 %
Aggregate 57 % 43 % 100 %Proportion
Property Cement Water
Specific Gravity 3.15 1.0
V = 1 ft
= 0.0347 ft
0 7279 0 1598 0 0776 . . .
= 0.0347+ 0.1598 = 19.45 %
e = V
= (0.0347+ 0.1598)/(0.7279+ 0.0776) = 0.24
alculated Air Content:
A = ft
n V V
V V V V V
V V ft
s a w s c
/ . / .
( )[ ]
= + +
1 0 100
100 0 0347 1 0 100
Unit Volume(1 ft3)
127.17 lb15.26 lb0.00 lb
Total 152.40 lb1.0 ft3
Figure 3. Constituent weight and volume distribution of RCC mixturebased on soil mechanics definitions.2
There are important differences between soil mechanics propertiesand the properties used in concrete practice. For example, there areseveral different ways to calculate the specific gravity. The specificgravity of the solid particles of the soil, not including the void spaces,is called the true or absolute specific gravity, which usually rangesbetween 2.6 to 2.7 for most soil. This is different from the apparentspecific gravity (dry weight) used in soil mechanics for compaction asdescribed above, and the saturated surface dry specific gravity used inconcrete mixture proportioning. Some of the resulting differences inproperties are demonstrated in the next section.
Proportioning RCC by Volumetric Method. Concrete proportioning can be performed by both weight and volumetric methods. Volumetricproportioning is performed using the specific gravity of each ingredient
to calculate the absolute volume that will be occupied in a unit volumeof concrete. The volumetric method is the more accurate method ofproportioning and is used for illustration purposes in this publication.
The absolute volume used in concrete mixture proportioning is based on the saturated surface dry specific gravity. The specific gravity,saturated surface dry (Gssd), is the ratio of the weight in air of a unit volume of aggregate, including the weight of water in the voids, comparedto the weight in air of an equal volume of water. The volume (yield) offreshly mixed concrete is the sum of the absolute volumes of the cementi-tous material (cement, pozzolan), aggregates, water (exclusive of thatabsorbed in the aggregate), admixtures, and air. The absolute volumes ofthe constituents (based on the volumetric method of mix proportioning) arecalculated using the material weight and specific gravity as shown below:
The specific gravity or relative density of the aggregate used in mixproportioning design can be based on either saturated surface dry(SSD) or oven dry materials. For the following example the Gssd, and amixture with the same total unit weight as Example 1, is used.
Example 2: A no-slump concrete mix consists of 3,491.70 pcy ofaggregate (saturated surface dry) with 57 % coarse aggregate, 412pcy of cement, and a water to cement ratio of 0.5124 (note for pur-poses of the example problem that the water cement ratio used hereinwas carried to more significant digits than is typical in concrete practice).The same material used in Example 1 will be used in Example 2. Themixture proportions including unit weights, absolute volumes, and aircontent are calculated on the next page.
Weight of material Specific gravity of material Unit weight of water
Calculate unit weights for each of the constituents for a one yd3 batch:
Cement = 412 lb
Water = 412 lb 0.5124= 211.10 lb
Coarse Aggregate(SSD) = (3,491.70 lb 57 %)
= 1,990.27 lb
Fine Aggregate(SSD) = 3,491.70 lb
= 1,501.43 lb
1990 27, . lb
The absolute volumes of the mix constituents are then calculated bydividing the known weight of each constituent by the product of itsspecific gravity and the unit weight of water.
Water =211.10 lb
1 62.4 pcf
3.15 62.4 pcf = 2.10 ft
Coarse Aggregate =1,990.27 lb
2.63 62.4 pcf ft
Fine Aggregate =1,501.43 lb
2.85 62.4 pcf
otal volume of known constituents:
= .38 ft 2.10 ft 12.13 ft 8.44 ft = 6.05 ft3 3 3 3 3
3 2+ + +
Next is to compare the different engineering properties used forconcrete mixture proportions with the properties defined in soilmechanics. Figure 4 shows a side-by-side comparison of the calcula-tions. The mix proportions are converted from 1 yd3 to 1 ft3 below,for comparison with the soil mechanics computations.
VolumeConstituent yd3 ft3
Water 3.38 0.1252Cement 2.10 0.0778Coarse Aggregate (ssd) 12.13 0.4492Fine Aggregate (ssd) 8.44 0.3126Air 0.95 0.0352 Check Sum 27.00 1.0000
Weight (lb)Constituent yd3 ft3
Water (Free water 211.10 7.82 above ssd)Cement 412.00 15.26 Coarse Aggregate (ssd) 1,990.27 73.71Fine Aggregate (ssd) 1,501.43 55.61 Air 0.0 0.0 Sum 4,114.80 152.40
The total water content (oven dry) and free water content (SSD) ofthe RCC mix can then be calculated, as shown on the next page.
Calculate air content:
= 7.00 ft ft ft
= 0.95 ft ft %
3 3 3
2 26 05 0 95
27 00 3 52
/ . .
Unit Volume(1 ft3)
15.26 lb0.00 lb
Total 152.40 lb1.0 ft3
Unit Volume(1 ft3)
Solids (SSD)Includes Absorbed
127.17 lb 15.26 lb0.00 lb
Total152.40 lb 1.0 ft3
(1.09 + 1.06 lbabsorbed)
Figure 4. Comparison of constituent distribution based on soil mechanics definitions and concrete volumetric proportions.
Roller-Compacted Concrete Density
Dry weight of
fine aggregate: = 55.61 lb
Dry weight of
total aggregate: = 72.62 lb 54.55 lb= 127.17 lb
Total water content: =7.82+1.09+1.06
Free water content: =7.82
1 06 54 55
It is clear from the examples above that there are some variations in thecalculated air content (3.47 % in soil mechanics versus 3.52% in con-crete methodology) and water content (7.0 % oven dry water contentfollowing soil mechanics versus 5.5 % free water and 7.0% oven drywater content for concrete volumetric proportioning). The differences areprimarily accounted for by the application of the definitions by the differ-ent practices (such as the specific gravity, water content, and water:cementratio that is used for proportioning aggregate content, and proportioningaggregate as a percentage of saturated surface dry aggregate), androunding of significant digits. The example problems demonstrate theimportance of distinguishing between the terms used in soil mechanicsand concrete practice (e.g. the total (oven dry) water content versus freewater content), and in the communication of mix proportions in laborato-ry programs, design and specifications, mixing plants, and field testing.The properties for both methodologies should be determined and docu-mented in the project record.
As mentioned earlier RCC placed at optimum moisture content(ASTM D 1557) contains a higher air content than is typicallyachieved in field placement and compaction.
Using the procedures shown in Examples 1 and 2, engineering prop-erties at different water contents can be used to further evaluateRCC mixtures. Six different water contents were evaluated for theexample material, corresponding to the six modified Proctor com-pactions test points as shown in Table 2. Evaluation of the engineer-ing properties in Table 2, shows that the minimum void ratio occursat the optimum moisture content. However, the air content of the
Free water = 7.82 lb
Absorbed water in
coarse aggregate: = 73.71 = 1.09 lb
Dry weight of
coarse aggregate: = 73.71 lb
Absorbed water in
fine aggregate: = 55.61 lb lb
(1+0.0195)= 1.06 lb
73 711 0 015
1 09 72 62
mixture continues to decrease in the compaction test until a pointapproximately 1 % over optimum. Placement of RCC at optimummoisture content and maximum density would be expected to resultin an air content of the compacted mix of about 3.5 %. In practice,most specifications accept a minimum compactive effort of 98 % ofthe maximum density resulting in a higher air content (5.5 %), forthe material in that example. Lower entrapped air content providesmore desirable hardened RCC properties. Also it is easier to compactslightly wetter mixtures. Therefore, for this example, selection of a mix ata water content that is 0.5 % to 1 % above optimum moisture contentwould provide the best opportunity for a workable, high density, lowair content mixture. For actual application of RCC in a project, themixture proportions shown above would be re-proportioned to a mix that would yield an air content of 2 % or lower (an example ofre-proportioning is shown in Appendix A in the Design Manual forRCC Spillways and Overtopping ProtectionPCA 2002).
The modified Proctor compaction test can be an efffective method ofselecting a water content that is both workable in the field and suit-able to meet the required RCC field properties Another benefit ofthe modified Proctor test for field control is that changes in basicmaterial properties automatically change the compaction curve.Frequent measurement of the specific gravity, gradation and absorptionduring construction will also allow adjustments of the mix propor-tions to accommodate changes as they occur.
There are numerous methods for the preparation of cylinders at thelaboratory stage that have been shown to be representative of actu-al field placement conditions. Cylinder preparation procedures thathave been used include: a) 10-ton vibratory roller (cores), b) Hilti orKango vibrating hammer, c) pneumatic tamper, d) Vebe table, e)internal vibrator, f) internal rodding, and g) Proctor test. The effec-tiveness of the different methods of cylinder preparation variesdepending on the workability of the RCC mixture. The effectivenessof each method (represented as a percentage of the maximumachievable strength) over the approximate range of moisture content(in excess of the SSD aggregate condition) is shown in Figure 5.
The pros and cons of each of the cylinder preparation methods aresummarized below:
Certainly the use of a full-scale roller (i.e., 10-ton vibratoryroller) would provide a close representation of actual fieldplacement conditions. However this method would requirelarge quantities of material, a large work area, and the use ofequipment not readily available at testing laboratories, fol-lowed by coring after a time delay, to obtain samples for test-ing. Consequently this method is generally impractical exceptfor large projects where test sections are often required.
The Hilti/Kango hammer method can also be used for a mod-erate range of mixture workability. This method has the advan-tage of using equipment (see Figure 6) that is readilyavailable, quite useable by laboratory personnel, and withamplitude and frequency very similar to normal field compaction
Table 2 Summary of Engineering Properties at Modified Proctor Compaction Points
Relative to Optimum Moisture - 3 % - 1 % Optimum Moisture + 0.5 % + 1 % + 2 %
Water Content 4 % 6 % 7.0 % 7.5 % 8 % 9 %
Dry Density 139.13 pcf 139.53 pcf 142.43 pcf 141.12 pcf 139.72 pcf 138.17 pcf
Porosity, n 21.4 % 21.2 % 19.5 % 20.3 % 21.1 % 21.9 %
Void Ratio, e 0.2720 0.2684 0.2422 0.2539 0.2666 0.2810
Wet Density 144.70 pcf 147.90 pcf 152.40 pcf 151.70 pcf 150.90 pcf 150.60 pcf
Water Content (Free water) 93.62 pcy 169.12 pcy 211.10 pcy 228.21 244.89 pcy 279.54 pcy
Water:Cement ratio1 0.2272 0.4107 0.5124 0.5539 0.5944 0.6785
Entrapped air content 12.5% 7.75 % 3.52 % 3.14 % 2.01 % 3.29 %
Note: 1. Water to cement ratio is based on a cement content of 412 pcy.
Cement = 175 pcyMax. aggregate = 11/2 in.
00 1 2 3 4 5 6 7 8
Free water content
Suitable rangefor various
Vebe = 120Vebe = 84
Vebe = 34
Vebe = 21
Vebe = 11
Vebe = 3
Vebe = 0
Slump = 0
Slump = 0.4 in.
Slump = 2.4 in.
Slump = 4.7 in.10 Ton vibrator roller
Laboratory Compaction Method and Free Water Contentvs.
Maximum Achievable Strength
Figure 5. Cylinder preparation method versus relative workability range. (It must be noted that the curve above is based on conventionalconcrete definitions using the free water content, i.e. the moisture content not including water absorbed in the aggregate. The actual,oven dry, water content would be higher when the total waterabsorbed plus free wateris included.) Ref 8.
equipment. A standard test procedure (ASTM C 1435) providesrepeatable results; however, depending on the mix design,compacted densities may be less then that achieveable in thefield. The method specifies placement of the material in threelifts, similar to the standard concrete test for rodding cylindersof slump concrete. However, RCC is a no-slump concrete withvery low workability. As a result the number of lifts may needto be increased to four or five to provide a cylinder that wouldbe expected to be similar to normal field compaction.
The pneumatic tamper (see Figure 7) can be used for a moderaterange of mixture workability. It is readily available at constructionsites, can be easily rented for laboratory use, and has beenshown to provide RCC cylinder densities that are similar toactual field conditions. The pneumatic tamper requires equip-ment not commonly used by laboratory personnel, and theamplitude and frequency are significantly different than withnormal field compaction equipment. Also there are no ASTMstandard test procedures available.
Roller-Compacted Concrete Density
Figure 6. Vibrating hammer used to prepare RCC cylinder (ASTM C 1435).
that is generally 10 to 15 pounds per cubic foot lower than the wetdensity. In general the wet density will remain constant throughoutthe chemical reaction (curing) process. While RCC does behave as a soil or granular base type material when it is first placed, theoptimum water content from the modified Proctor test is typicallyless than required for full compaction (consolidation) of the RCC.The result is placement to the maximum dry density at optimumwater content will generally result in more entrapped air voids thanconventional concrete.
There are several methods that have been successfully used as compaction standards for RCC compaction control. The primarymethods are: 1) theoretical air-free density, 2) field/laboratory cylin-der density, and 3) average maximum density. These methods cangenerally be described as follows:
Theoretical Air-Free Density (TAFD) Standard Thismethod consists of a theoretically calculated density of an RCCmix based on the mass properties (specific SSD gravity andabsorption). One factor that causes variations in the calculatedwet density of the RCC is the percent of air contained within asample of RCC, which can be difficult to accurately measureunder field conditions. The percent of air measured in thor-oughly compacted RCC mixes has typically ranged between0.5 % and 2 %. Use of a percentage of the theoretical air-freedensity as a compaction control density eliminates this vari-ability. Therefore measurement of the air content in the fieldwould be academic. When differences in the field measureddensity and the TAFD are noted, it is more often due to varia-tions in the aggregate proportions, which can be readily moni-tored by gradation analysis, or aggregate properties, such asthe specific gravity and/or absorption of the material that maychange throughout construction. The required compactionstandard by this method usually ranges from 96 % to 98 % ofthe TAFD, with no individual test below 95 % of the TAFD.
Ongoing aggregate testing and mixing plant production duringconstruction can be readily performed to monitor for changesin the proportions and/or properties. If variations are noted,the TAFD can be adjusted accordingly. This process is similar toperforming gradation tests and compaction curves for conven-tional earthfill projects.
Cylinder Density Standard Compaction control usingcylinders compacted in the field or laboratory is based onmeasuring the average wet unit weight of standard 6 x 12inch cylinders constructed of the RCC mix. As discussed above,the cylinders can be fabricated by the vibrating hammermethod (ASTM C 1435), Vebe method (ASTM C 1176), modi-fied Proctor (ASTM D 1557), or the use of a pneumatic tamper(which does not have a standardized test method). Test cylindersprepared by these four methods have been found to closelyapproximate the in-place density of RCC compacted underfield conditions. When the cylinder density closely approxi-mates the in-place field density, the compressive strength ofthe RCC cylinder can accurately approximate the compressivestrength of the in-place compacted RCC. A metal mold should
Cylinders prepared with the Vebe table method (see Figure 8)have also been shown to be similar to normal field com-paction for mixes with a Vebe time of 35 seconds or less. Astandard test procedure (ASTM C 1176) provides repeatableresults. Experience has shown that the Vebe method works for anarrower range of mix workability than the pneumatic tamper orHilti/Kango methods.
Internal vibrators/rodding are not used for the preparation ofRCC cylinders. These two methods are primarily suitable forslump concrete, and external compaction equipment used forRCC cannot operate effectively or efficiently on slump concrete.
The modified Proctor compaction test is also an effective cylinder preparation method that represents normal field compaction. A test procedure (ASTM D 1557) provides arepeatable standardized method. The modified Proctor testactually covers a wider range of mixture workability than istypically employed by any other method. However, applicationof the modified Proctor test in the field is not practical due tothe amount of time and labor required to prepare the cylinders fortesting. Any delay in casting the standard 6-inch diameter cylinderscan allow the mixture workability and properties to change due tocement hydration and evaporation loss.
Wet density is the most widely used method of reporting RCC densityand should be the primary control standard used in RCC construction.Dry density, used in standard geotechnical construction practice, mayprovide some useful reference information. However, in RCC prac-tice, one typically tries to achieve the fewest practical air voids thatwill occur at a higher water content than the maximum dry density,which is the objective used in typical geotechnical engineering practice.The difference between concrete practice and geotechnical practice generally follows from the fact that as RCC hardens its in-place densityis reflective of the wet density of the material, not the dry density
be used to provide confine-ment and maintain therequired cylinder dimensionsduring compaction.
The required compactionstandard by the cylinder den-sity method is usually atleast 98 % of the averagecontrol cylinder density, withno individual test below 96% of the average controlcylinder density. Sinceentrapped air content isincluded in the results of allthese methods, the density val-ues will be less than the TAFD,by definition.
The vibrating hammer, Vebe, and modified Proctor test meth-ods benefit from the existence of established standards thatcan be used in the laboratory during the design phase as wellas for field control during construction. These test methods arerepeatable and easy to perform. In the case of the vibratinghammer and Vebe test, the methods have similar compactionproperties (frequency and amplitude of compaction) as fieldcompactors typically used for construction. The pneumatictamper, while showing good correlation with field compaction,has a significantly different amplitude and frequency of
Figure 8. Preparation of RCCcylinder using the Vebe Table.
Figure 7. Preparation of RCC using a pneumatic tamper.
compaction (which varies widely based on the reaction force provided by the operator) compared to typical com-paction equipment, and does not have a standardized testmethod.
Average Maximum Density (AMD) The AMD test methodinvolves the preparation in the field of a test section whereby theRCC is compacted with different compactors and various numbersof passes by the equipment, and the average maximum densityachieved (as measured by the nuclear density gauge) is used as acontrol standard. The maximum density used for compaction con-trol from a test strip is also sometimes referred to as the optimumcompaction density value (although this term can be confusedwith the optimum moisture content and maximum density derivedfrom the modified Proctor compaction test.) There are also severalvariations in terminology such as the maximum achievable densitythat are essentially developed in a similar manner. Based on theresults of the field test section, the required placement density isspecified as a percentage of the AMD. The standard for thismethod is similar to the development of a method specification forthe control of rockfill placement.
During development of a method specification for fill placement,a full range of density, moisture, gradation, and void content analy-ses (either measured or compared with the theoretical air-free den-sity) would also be expected to be performed. Therefore, moretesting than the measurement of the in-situ density in the test fillis necessary to ensure that the AMD is representative of therequired design conditions and not the result of the maximumdensity that can be achieved with an inappropriate compactorand/or a RCC mix that is too dry or too wet. The required compaction standard by this method is usually the average densityno less than 98 % of the AMD determined in the test strip, withno individual test below 96 %.
The use of the AMD method should be combined with the measurement of the TAFD, void content, uniformity of the RCCdensity by depth, and engineering properties that may vary duringconstruction (e.g., gradation, specific gravity, and absorption) thatwould require another test strip to establish a new AMD.
The end results of each method are actually quite similar. Using datafrom two actual constructed projects, the TAFD and cylinder densi-ties can be summarized and compared to the compaction standardmethods described above. Table 3 shows the TAFD, cylinder densi-ties, and field densities for two projects.
Density Method Project A Project B
Theoretical Air-Free Density (TAFD) 166.5 pcf 152.4 pcf
Cylinder Density 162.7 pcf 149.2 pcf
Field Density (average of tests 162.8 pcf 146.9 pcfduring construction)
Table 3 Example Data for Compaction Standards
Roller-Compacted Concrete Density
Using the data in Table 3, a comparison can be made of the com-paction standard with conditions achieved in field. Typically, specifi-cations using the TAFD as the compaction standard will require thatfield compaction achieve a minimum of 96 % of the TAFD. Usingthe example projects shown in Table 3, the field compaction stan-dard density requirement for the two projects would be 159.8 pcfand 146.3 pcf as shown in Table 4, below.
Table 4 Theoretical Air-Free DensityCompaction StandardCompaction Standard Project A Project B
Required Field Compaction Standard 159.8 pcf 146.3 pcf96 % TAFD
The actual field densities achieved during construction would meetthe 96 % TAFD compaction standard.
Typically, specifications using the cylinder density as the compactionstandard will require that field compaction achieve a minimum of 98 %of the average cylinder density. Using the example projects shown in Table 3, the field compaction standard density requirement for the two projects would be 159.4 pcf and 146.2 pcf as shown inTable 5, below.
Table 5 Cylinder Density Compaction StandardCompaction Standard Project A Project B
Required Field Compaction Standard 159.4 pcf 146.2 pcf98 % of Cylinder Density
Therefore, a similar objective is met using either of these compactionstandards, and both methods have applicability of use in the labora-tory and field. The field density tests for both example projects showthat RCC can be compacted to an acceptable compaction standard.
Use of a test strip in the field as the compaction standard is muchmore subjective than the other methods described herein. For exam-ple, if the compactor used in a test strip is too light, the dynamicproperties (frequency and/or amplitude) are not suitable for the RCCmix being used, or the mix is too dry or too wet, an AMD can still bedeveloped. However, the result may be that the RCC placed mayhave a high enough void content that the strength, permeability,and/or durability could fall below the design objective or laboratorytests used for design. Therefore extra care and experience are neededwhen using the AMD method to establish a compaction standard.In all cases, knowing the air content of an RCC mixture (using theconcrete practice definition) is critical to understanding the densityof the in-place material, and it is important to use the extensive history of concrete strength, permeability, and durability whenassessing the in-situ conditions of RCC.
Historically, different methods have been successfully used to establish adensity standard for RCC placement during construction. Under projectspecific circumstances, some methods to control compaction and estab-lish a maximum or target density may be more applicable than others.The most important objective in establishing a compaction standard forconstruction of RCC is to select a method that simulates the field condi-tions under which the RCC is being compacted and has a basis ofrepeatability and uniform application (of benefit to a contractor). Thecompaction method and method of arriving at the field target densityshould always be clearly described in construction documents.
Materials properties and mixture proportions should be clearly and completely defined. A complete listing of all of the properties(soil mechanics and concrete methodology) will greatly enhancecommunication and data interpretation and reduce the potential formisinterpretation of or confusion about the properties specified.
The author, Terry Arnold, Senior Principal Engineer, MWH (MontgomeryWatson Harza) Americas Inc. would like to express his gratitude to:Randy Bass, Water Resources Manager, and Wayne Adaska, Directorof Public Works, Portland Cement Association; Dan Johnson, DeputyDirector, Domestic Hydropower and Dams, Global Energy & Industry,Inc., and Mike Miller, Principal Engineer, MWH Americas Inc., fortheir invaluable contributions in the preparation of this document.
1. T.W. Lambe and R.V. Whitman, Soil-Mechanics, John Wiley &Sons, 1969.
2. M.G. Spangler and R.L. Handy, Soil Engineering Handbook,Third Edition, 1973.
3. T.J. Casias, V. D. Goldsmith, and A. A. Benevidez, SoilLaboratory Methods Applied to RCC, proceedings, AmericanSociety of Civil Engineers, Roller-Compacted Concrete IIConference, February 1988, pp.107122.
4. T. Arnold, T. Feldsher, and K. Hansen, RCC Test SpecimenPreparations: Developments Toward a Standard Method,proceedings, American Society of Civil Engineers, Roller-Compacted Concrete III Conference, February 1992, pp.341357.
5. N.C. Wong, J.A. Bischoff, and D. H. Johnson, Strengtheningand Raising Gibraltar Dam with RCC, proceedings, AmericanSociety of Civil Engineers, Roller-Compacted Concrete IIConference, February 1988, pp. 236250.
6. G. N. Reeves and L. B. Yates, Jr., Simplified Design andConstruction Control for Roller-Compacted Concrete, pro-ceedings, American Society of Civil Engineers, Roller-CompactedConcrete II Conference, May 1985, pp.4865.
7. H. Winterkorn, J. Hilf, and H.Y. Fang, Foundation EngineeringHandbook, Chapter 7, Compacted Fill, Van Nostrand ReinholdCompany, 1975.
8. Schrader, E. K., Appropriate Laboratory Compaction Methodsfor Different Types of Roller-Compacted Concrete (RCC),proceedings, 4th International Symposium on Roller-CompactedConcrete Dams, Madrid, Spain, November 17-19, 2003.
Roller-Compacted Concrete Density
Note: This document is written in English units. To convert to metric units use the conversion table presented below:
To Convert Into Multiply By
Inch (in.) Millimeter (mm) 25.4
Foot (ft) Meter (m) 0.3048
Square foot (ft2) Square meter (m2) .0929
Square yard (yd2) Square meter (m2) 0.8361
Cubic foot (ft3) Cubic meter (m3) 0.02832
Cubic yard (yd3) Cubic meter (m3) 0.7646
Pound (lb) Kilogram (kg) 0.4536
Pound per square inch (psi) Kilopascal (kPa) 6.8948
Pound per cubic foot (pcf) Kilogram per cubic meter (kg/m3) 16.0185
Pound per cubic yard (pcy) Kilogram per cubic meter (kg/m3) 0.5933
Portland Cement Association ("PCA") is a not-for-profit organization and provides this publi-cation solely for the continuing education of qualified professionals. THIS PUBLICATIONSHOULD ONLY BE USED BY QUALIFIED PROFESSIONALS who possess all required license(s),who are competent to evaluate the significance and limitations of the information providedherein, and who accept total responsibility for the application of this information. OTHERREADERS SHOULD OBTAIN ASSISTANCE FROM A QUALIFIED PROFESSIONAL BEFORE PROCEEDING.
PCA AND ITS MEMBERS MAKE NO EXPRESS OR IMPLIED WARRANTY WITH RESPECT TO THISPUBLICATION OR ANY INFORMATION CONTAINED HEREIN. IN PARTICULAR, NO WARRANTYIS MADE OF MERCHANTABILITY OR FITNESS FOR A PARTICULAR PURPOSE. PCA AND ITSMEMBERS DISCLAIM ANY PRODUCT LIABILITY (INCLUDING WITHOUT LIMITATION ANYSTRICT LIABILITY IN TORT) IN CONNECTION WITH THIS PUBLICATION OR ANY INFORMATIONCONTAINED HEREIN.
This publication is intended SOLELY for use by PROFESSIONAL PERSONNEL who are compe-tent to evaluate the significance and limitations of the information provided herein, and whowill accept total responsibility for the application of this information. The Portland CementAssociation DISCLAIMS any and all RESPONSIBILITY and LIABILITY for the accuracy of and theapplication of the information contained in this publication to the full extent permitted by law.
An organization of cement companies toimprove and extend the uses of portlandcement and concrete through market development, engineering, research,education, and public affairs work.
2004 Portland Cement Association.All rights reserved.
Click here to load reader